Optimizing the Catalytic Performance of Ba1−xCexMnO3 and Ba1−xLaxCu0.3Mn0.7O3 Perovskites for Soot Oxidation in Simulated GDI Exhaust Conditions

Ba1−xCexMnO3 (BM-Cex) and Ba1−xLaxMn0.7Cu0.3O3 (BMC-Lax) perovskite-type mixed oxides were synthesized using the sol–gel method adapted for aqueous media with different values of x (0, 0.1, 0.3, 0.6) to estimate the effect of the degree of the partial substitution of Ba by Ce or La on the structure and properties that are relevant for their use as catalysts for gasoline direct injection (GDI) soot oxidation. The samples were deeply characterized by ICP-OES, XRD, XPS, N2 adsorption, H2-TPR, and O2-TPD, and their potential as catalysts for soot oxidation has been analyzed in various scenarios that replicate the exhaust conditions of a GDI engine. By comparing the catalytic performance for soot oxidation of the two tested series (BM-Cex and BMC-Lax) and in the two conditions used (100% He and 1% O2 in He), it could be concluded that (i) in the absence of oxygen in the reaction atmosphere (100% He), BMC-La0.1 is the best catalyst, as copper is also able to catalyze the soot oxidation; and (ii) if oxygen is present in the reaction atmosphere (1% O2/He), BM-Ce0.1 is the most-active catalyst as it presents a higher proportion of Mn(IV) than BMC-La0.1. Thus, it seems that the addition of an amount of Ce or La higher than that corresponding to x = 0.1 in Ba1−xCexMnO3 and Ba1−xLaxCu0.3Mn0.7O3 does not allow us to improve the catalytic performance of BM-Ce0.1 and BMC-La0.1 for soot oxidation in the tested conditions.


Introduction
Perovskite-type mixed oxides (with the general formula ABO 3 ) are becoming increasingly popular in the materials science and catalysis fields due to their tunable properties [1][2][3][4].The unique crystal structure, the non-stoichiometry in oxygen, the acid-base and redox properties, and the thermal stability enable perovskites to be effective as catalysts for different reactions, including, among others, oxidation, hydrogenation, and photocatalytic reactions [1][2][3][4].Moreover, perovskites are also being employed for electrocatalytic applications as solid oxide fuel cells due to their oxygen-ion-conducting properties [5].Considering the main topic of the present work, perovskite-type oxides are being used as catalysts in the process related to the post-treatment of car exhaust gases, such as carbon monoxide, hydrocarbon and/or soot oxidation, and NO x reduction [1,3,4,6].Focusing our attention on soot oxidation, this application has become relevant in recent years as GDI engines are considered as a novel option which ensures a higher fuel economy and lower pollutant emissions compared with the traditional port fuel injection engines [7].Regarding perovskites, it is generally accepted that their catalytic activity for soot oxidation is related to the presence of oxygen vacancies, to the oxygen's mobility through the solid, and to the redox properties [1,4].Additionally, it has been proved that modifications on some physical properties of perovskites, such as particle size, surface area, morphology, and crystal structure, as well as composition, affect the catalytic performance [6,8].Considering the composition of perovskites, it has been demonstrated that the incorporation of cerium and lanthanum in the A-site of ABO 3 perovskites improves the catalytic performance of these oxides by promoting the creation of oxygen vacancies and by enhancing the redox properties, and thus the mobility, of oxygen [9][10][11][12][13][14][15].In particular, some perovskites based on Ba 0.9 A 0.1 MnO 3 and Ba 0.9 A 0.1 Mn 0.7 Cu 0.3 O 3 (A = Mg, Ce, La, Ca, Sr) formulations have been previously employed as catalysts for soot oxidation in simulated GDI engine exhaust conditions [16], and researchers have concluded that Ba 0.9 Ce 0.1 MnO 3 is the most active in 1% O 2 /He (being T 50% = 641 • C, which is the temperature for achieving 50% of soot oxidation versus 710 • C for BaMnO 3 raw perovskite), while Ba 0.9 La 0.1 Cu 0.3 Mn 0.7 O 3 presents the best performance in the absence of oxygen (T 10% = 611 • C, which is the temperature for achieving 10% of soot oxidation versus 879 • C for BaCu 0.3 Mn 0.7 O 3 perovskite).However, as the content of cerium or lanthanum could be relevant for the catalytic performance [17], the goal of this work is to evaluate the influence of the degree of cerium and lanthanum substitution on the properties of Ba 1−x Ce x MnO 3 (denoted as BM-Cex) and Ba 1−x La x Cu 0.3 Mn 0.7 O 3 (named as BMC-La x ) (x = 0, 0.1, 0.3, 0.6) perovskite-type mixed oxides that determine their use as catalysts for GDI soot oxidation.

Results and Discussion
2.1.Catalysts Characterization 2.1.1.Ba 1−x Ce x MnO 3 (x = 0, 0.1, 0.3, 0.6) Table 1 shows the nomenclature and the actual cerium content (wt%) determined using Inductively Coupled Plasma Optical Emission Spectroscopy (ICP-OES) and the Brunauer-Emmett-Teller (BET) surface area.As a reference, the data corresponding to the raw BaMnO 3 (BM) perovskite have been included.First, as expected, the cerium percentage increases with the degree of substitution, ranging from 1.3 wt% to 6.0 wt%.The samples present low BET surface areas, as is usual for perovskite-type mixed oxides [1,18,19], because the porosity was not well developed during the synthesis, probably due to the relatively high calcination temperature used (850 • C) [20,21].
In the X-ray diffraction (XRD) patterns of BM-Cex perovskites (Figure 1), diffraction peaks at c.a. 2θ 25.8 • , 31.4 • , 41.1 • , 52.8 • , 55.9 • , and 65.7 • , corresponding to the hexagonal 2H-BaMnO 3 perovskite structure (PDF number: 026-0168, designated by the International Centre of Diffraction Data, ICDD), are identified.As the percentage of Ce in the composition of perovskites increases, the intensity of the peaks corresponding to the hexagonal perovskite structure decreases, being replaced by peaks at c.a. 28.6 • , 33.2 • , 47.5 • , and 56.5 • 2θ values (PDF numbers: 43-1002) corresponding to CeO 2 .In fact, for BM-Ce 0.6 , this phase becomes the main one, while it is a minority phase for BM-Ce 0.1 .On the other hand, only MnO 2 (PDF numbers: 024-0735) was detected as a minority phase for BM, BM-Ce 0.1 , and BM-Ce 0.3 , being the relatively low calcination temperature used during the sol-gel synthesis (850 • C), which is probably responsible for its presence.Thus, the intensity of the main XRD peak for the hexagonal perovskite structure increases for BM-Ce 0.1 with respect to BM.However, at higher values of x, the intensity decreases in favor of the CeO 2 crystalline phase, which increases until becoming the most intense peak for BM-Ce 0.6 .The average crystallite size displayed in Table 2 was calculated by applying the Williamson-Hall method to the XRD peaks of hexagonal-2H-BaMnO 3 phase [22], and a decrease is observed in the presence of cerium in favor of CeO 2 phase.Finally, the values calculated for "a" and "c" cell parameters for the hexagonal structure, as depicted in Table 2, closely resemble those of the reference sample (BM); so, it seems that the incorporation of Ce into the perovskite network does not modify these parameters, as cerium appears as CeO 2 , avoiding the modification of the BaMnO 3 structure.The described trend of the different crystalline phases with respect to the Ce percentage is confirmed by the XRD refinement data shown in Table 2.
Molecules 2024, 29, x FOR PEER REVIEW 3 of 21 crystallite size displayed in Table 2 was calculated by applying the Williamson-Hall method to the XRD peaks of hexagonal-2H-BaMnO3 phase [22], and a decrease is observed in the presence of cerium in favor of CeO2 phase.Finally, the values calculated for "a" and "c" cell parameters for the hexagonal structure, as depicted in Table 2, closely resemble those of the reference sample (BM); so, it seems that the incorporation of Ce into the perovskite network does not modify these parameters, as cerium appears as CeO2, avoiding the modification of the BaMnO3 structure.The described trend of the different crystalline phases with respect to the Ce percentage is confirmed by the XRD refinement data shown in Table 2.  Corresponding to hexagonal-2H-BaMnO3, except for BM-Ce0.6,which corresponds to CeO2.b Calculated using the Williamson-Hall method for the XRD peaks of hexagonal 2H-BaMnO3 (around 2θ = 26°, 32°, and 41°), except for BM-Ce0.6,which corresponds to CeO2 (around 2θ = 29°, 31° and 33°) due to the low intensity of the hexagonal perovskite peaks.c Calculated using the main perovskite XRD peak of the BaMnO3 hexagonal structure (2θ = 32°).) due to the low intensity of the hexagonal perovskite peaks.c Calculated using the main perovskite XRD peak of the BaMnO 3 hexagonal structure (2θ = 32 • ).
To determine the surface composition and oxidation states of the elements present on the surface of samples, the X-ray photoelectron spectroscopy (XPS) technique was employed (see the Materials and Methods section for details), and the most relevant findings are shown in Figure 2 and Table 3.The XPS spectra for the O 1s transition (Figure 2a) show three peaks at c.a. 529.1, 531.1, and 532.7 eV, attributable to lattice oxygen (O L ), absorbed oxygen species (O ads ) that include surface carbonate (CO 3 −2 ), hydroxyl groups (OH − ), peroxide (O 2 −2 ) or superoxide (O −2 ) ions and defect sites with low oxygen coordination (oxygen vacancies), and, finally, adsorbed water species (O H2O ) [23][24][25].By comparing with raw BM perovskite, the binding energy (BE) corresponding to the maximum of O ads peaks shifted towards lower values with the increase in the cerium content due to the presence of more oxygen species (from CeO 2 ) on the surface [26], while no significant shift is detected in BE max for O L .As the O L /(Ba + Ce + Mn) ratio (calculated using the area under the O L peak and the area of the peaks for cations present on surface) is lower than the theoretical value for perovskites (1.5), oxygen vacancies are present on the surface of all samples, and, as the values rise from 1 to 1.2, an increase in the amount of lattice oxygen species occurs, which seems to be due to the presence of the CeO 2 .Temperature-programmed reduction tests with H2 (H2-TPR) were used to evaluate the reducibility of BM-Cex mixed oxides, as the reducibility is related to its activity in the oxidation process [38].Figure 3a shows the hydrogen consumption profiles of BM and BM-Cex perovskites, as well as the corresponding MnO2 used as a reference.The H2-TPR profile for MnO2 shows two main reduction peaks with maxima at around 400 and 500 °C.The first main reduction peak (at ∼400 °C) is associated with the reduction of MnO2 and/or Mn2O3 to Mn3O4; whereas the second main peak (at ∼500 °C) is assigned to the reduction of Mn3O4 to MnO [38].The H2-TPR profiles of BM and all BM-Cex samples exhibit three reduction peaks: (i) the first one, in the temperature region between around 300 and 600 °C, corresponds to the reduction of Mn(IV)/Mn(III) to Mn(II), as well as, for Cedoped samples, to the reduction of surface Ce(IV) to Ce(III) [31,36]; (ii) in the intermediate temperature region (between 600 and 800 °C), the observed peak is linked to the desorption/reduction of oxygen species and to the reduction of the CeO2 bulk phase [39] for cerium-doped samples; and, finally, (iii) the very-low-intensity peak at the highest temperature region (between 900-1000 °C) is associated with the reduction of bulk Mn(III).After doping with Ce, the main reduction peak (with a maximum at around 500 °C) is slightly shifted towards lower temperatures with respect to the undoped BM perovskite (482 °C versus 468, 442, and 457 °C for BM-Ce0.1,BM-Ce0.3, and BM-Ce0.6,respectively); so, the reduction of Mn/Ce takes place at a lower temperature for the doped samples, probably due to a synergetic effect between Mn and Ce [40].The experimental hydrogen consumption per gram of catalyst, calculated between 200 °C and 600 °C (using the hydrogen consumption patterns illustrated in Figure 3a, is compared in Figure 3b with the hydrogen  According to the literature, the assignment of the manganese oxidation states via XPS is a difficult task [27][28][29][30][31]; however, the raw data for Mn 2p 3/2 spectra suggest the presence of Mn (III) and Mn (IV).Considering the asymmetric shape of the XPS signal, and based on the analysis of Ponce et al. for manganese-based perovskites [32], the two components of the Mn 2p 3/2 spectra (Figure 2b) could be interpreted as follows: the deconvoluted peak at BE = 641.4-640.6 eV corresponds to Mn(III), and the observed peak at BE = 642.5-642.1 eV to Mn(IV).The presence of the satellite peak of Mn(III) at a binding energy of c.a. 644 eV allows us to confirm that Mn(III) exists on the surface.For BM-Ce 0.3 and BM-Ce 0.6 samples, a slight shift towards lower binding energies of Mn(III) with respect to BM and BM-Ce 0.1 peak can be observed, which should be related to the increased amount of CeO 2 detected via XRD.Thus, these spectra reveal that Mn(III) and Mn(IV) coexist on the surface of all perovskites [30,31,33], as these oxidation states allow for the surface to become electroneutral.Note also that for most of samples, Mn(III) shows two deconvolutions that reveal two different electronic environments, probably originating in the presence of oxygen vacancies and/or in the existence of Ce in different oxidation states, as it will be discussed below.The Mn(IV)/Mn(III) ratio values (calculated using the area under the corresponding deconvoluted XPS peaks and summarized in Table 3) decrease as the cerium percentage increases; so, the presence of cerium promotes an increase in Mn(III) on the surface with respect to Mn(IV), with this fact also being related to the electroneutrality (as Ce(IV)/Ce(III) is replacing Ba(II) in the perovskite formulation).Thus, Mn(IV) is the main oxidation state on the surface for BM and BM-Ce 0.1 , but it is Mn(III) for the other two samples with higher cerium percentages.Note that BM-Ce 0.6 does not follow this trend, as the Mn(IV)/Mn(III) ratio increases with respect to BM-Ce 0.3 .So, as the ratio is close to 1, the surface of this sample should present an almost-similar amount of both oxidation states.
Figure 2c illustrates the XPS spectra corresponding to the Ce 3d orbitals.According to relevant literature [34][35][36][37], the deconvolution of these spectra reveals eight sub-peaks: four v quadruplets within the Ce 3d 5/2 region and four u quadruplets within the Ce 3d 3/2 region.Within these sub-peaks, the Ce(III) oxidation state is discernible through the two specific subpeaks v 1 and u 1 , being the remaining sub-peaks associated with the Ce(IV) oxidation state.Thus, both Ce(III) and Ce(IV) are present on the surface of all BM-Ce x samples, but as the Ce(IV)/Ce(III) ratios are higher than 1, this means that the amount of Ce(IV) is higher than that of Ce(III).The presence of the two valences of Ce on the surface seems to be relevant as it could enhance the oxygen storage capacity [9].Moreover, as the Ce(IV)/Ce(III) ratio increases with the Ce percentage, the Ce(IV) proportion also increases from BM-Ce 0.1 to BM-Ce 0.6 .This finding agrees with the XRD data, which reveal the prevalence of CeO 2 in the bulk of samples as Ce content increases.
Temperature-programmed reduction tests with H 2 (H 2 -TPR) were used to evaluate the reducibility of BM-Cex mixed oxides, as the reducibility is related to its activity in the oxidation process [38].Figure 3a shows the hydrogen consumption profiles of BM and BM-Cex perovskites, as well as the corresponding MnO 2 used as a reference.The H 2 -TPR profile for MnO 2 shows two main reduction peaks with maxima at around 400 and 500 • C. The first main reduction peak (at ∼400 • C) is associated with the reduction of MnO 2 and/or Mn 2 O 3 to Mn 3 O 4 ; whereas the second main peak (at ∼500 • C) is assigned to the reduction of Mn 3 O 4 to MnO [38].The H 2 -TPR profiles of BM and all BM-Cex samples exhibit three reduction peaks: (i) the first one, in the temperature region between around 300 and 600 • C, corresponds to the reduction of Mn(IV)/Mn(III) to Mn(II), as well as, for Ce-doped samples, to the reduction of surface Ce(IV) to Ce(III) [31,36]; (ii) in the intermediate temperature region (between 600 and 800 • C), the observed peak is linked to the desorption/reduction of oxygen species and to the reduction of the CeO 2 bulk phase [39] for cerium-doped samples; and, finally, (iii) the very-low-intensity peak at the highest temperature region (between 900-1000 • C) is associated with the reduction of bulk Mn(III).After doping with Ce, the main reduction peak (with a maximum at around 500 • C) is slightly shifted towards lower temperatures with respect to the undoped BM perovskite (482 • C versus 468, 442, and 457 • C for BM-Ce 0.1 , BM-Ce 0.3 , and BM-Ce 0.6 , respectively); so, the reduction of Mn/Ce takes place at a lower temperature for the doped samples, probably due to a synergetic effect between Mn and Ce [40].The experimental hydrogen consumption per gram of catalyst, calculated between 200 • C and 600 • C (using the hydrogen consumption patterns illustrated in Figure 3a, is compared in Figure 3b with the hydrogen consumption calculated, assuming the entire reduction of Ce (IV) and Mn as either Mn(III) (blue line) or Mn(IV) (red line).For BM, it seems that Mn(IV) is the main oxidation state in the bulk, as the experimental value is close to the corresponding point in the red line.However, after doping with cerium, the experimental H 2 consumptions approach Mn(III) (and Ce(IV)), so Mn(III) seems to be the main oxidation state in the bulk of the BM-Cex samples.However, a decrease is observed from BM-Ce 0.1 to BM-Ce 0.6 , probably due to the increasing amount of bulk CeO 2 (as detected via XRD).
The mobility of O 2 for BM-Cex samples was investigated by analyzing the emission of O 2 during the temperature-programmed desorption of O 2 (O 2 -TPD) tests, and the O 2 evolution profiles are shown in Figure 4.The amount of O 2 released from perovskites was determined by the integration of the O 2 desorption profiles, using CuO as a reference [31] and assuming that CuO is converted to Cu 2 O [41,42].For perovskite-type mixed oxides, three types of oxygen are usually identified: α-O 2 , α'-O 2 , and β-O 2 .α-O 2 refers to oxygen that evolves from that adsorbed on the surface vacancies; α -O 2 corresponds to oxygen coming from that the adsorbed on the surface lattice defects, such as dislocations or grain borders; and finally, β-O 2 is the oxygen desorbed from the perovskite lattice [1,27,30], which is dependent on the partial reduction of Mn(IV) to Mn(III) [43,44], and also on the reduction of Ce(IV) to Ce(III) for BM-Cex samples [12], and whose desorption is facilitated by the presence of bulk oxygen vacancies.All BM-Cex samples evolve oxygen in the high-temperature region (β-O 2 ), and the amount evolved (calculated from the area under the O 2 profiles and using CuO as reference) increases from 114 µmol g −1 for BM-Ce 0.1 to 136 µmol g −1 for BM-Ce 0.3 , but it decreases to 98 µmol g −1 for BM-Ce 0.6 .So, the oxygen evolved is notably higher for BM-Cex samples (as BM only generates 23 µmol g −1 ), revealing an improved oxygen mobility through the perovskite lattice in the presence of Ce, probably due to the contribution of the Ce(IV)/Ce(III) redox pair.However, this trend is not followed by BM-Ce 0.6 , and this finding seems to be related to the decrease in the reducibility as the Ce content increases, as revealed by the H 2 -TPR results (Figure 3).Finally, the BM-Ce 0.1 sample shows a small desorption peak between 500 and 650 • C, which corresponds to the oxygen adsorbed on the surface lattice defects (α -O 2 ), which is highlighted in Figure 4.
Molecules 2024, 29, x FOR PEER REVIEW 7 of 21 consumption calculated, assuming the entire reduction of Ce (IV) and Mn as either Mn(III) (blue line) or Mn(IV) (red line).For BM, it seems that Mn(IV) is the main oxidation state in the bulk, as the experimental value is close to the corresponding point in the red line.However, after doping with cerium, the experimental H2 consumptions approach Mn(III) (and Ce(IV)), so Mn(III) seems to be the main oxidation state in the bulk of the BM-Cex samples.However, a decrease is observed from BM-Ce0.1 to BM-Ce0.6, probably due to the increasing amount of bulk CeO2 (as detected via XRD).The mobility of O2 for BM-Cex samples was investigated by analyzing the emission of O2 during the temperature-programmed desorption of O2 (O2-TPD) tests, and the O2 evolution profiles are shown in Figure 4.The amount of O2 released from perovskites was determined by the integration of the O2 desorption profiles, using CuO as a reference [31] and assuming that CuO is converted to Cu2O [41,42].For perovskite-type mixed oxides, three types of oxygen are usually identified: α-O2, α'-O2, and β-O2.α-O2 refers to oxygen that evolves from that adsorbed on the surface vacancies; α´-O2 corresponds to oxygen coming from that the adsorbed on the surface lattice defects, such as dislocations or grain borders; and finally, β-O2 is the oxygen desorbed from the perovskite lattice [1,27,30], which is dependent on the partial reduction of Mn(IV) to Mn(III) [43,44], and also on the reduction of Ce(IV) to Ce(III) for BM-Cex samples [12], and whose desorption is facilitated by the presence of bulk oxygen vacancies.All BM-Cex samples evolve oxygen in the hightemperature region (β-O2), and the amount evolved (calculated from the area under the O2 profiles and using CuO as reference) increases from 114 µmol g −1 for BM-Ce0.1 to 136 µmol g −1 for BM-Ce0.3,but it decreases to 98 µmol g −1 for BM-Ce0.6.So, the oxygen evolved is notably higher for BM-Cex samples (as BM only generates 23 µmol g −1 ), revealing an improved oxygen mobility through the perovskite lattice in the presence of Ce, probably due to the contribution of the Ce(IV)/Ce(III) redox pair.However, this trend is not followed by BM-Ce0.6, and this finding seems to be related to the decrease in the reducibility as the Ce content increases, as revealed by the H2-TPR results (Figure 3).Finally, the BM-Ce0.1 sample shows a small desorption peak between 500 and 650 °C, which corresponds to the oxygen adsorbed on the surface lattice defects (α´-O2), which is highlighted in  Table 4 lists the nomenclature, the La and Cu metal contents (obtained by ICP-OES), and the BET surface area of Ba1−xLaxMn0.7Cu0.3O3(BMC-Lax) samples.According to the ICP-OES data, the percentage of Cu ranges from 7.1 wt% for BMC-La0.6 to 9.8 wt% for BMC-La0.3,showing a wt% La from 5.4 wt% to 24.0 wt%.As seen in Table 4, the BET surface area 2.1.2.Ba 1−x La x Mn 0.7 Cu 0.3 O 3 (x = 0, 0.1, 0.3, 0.6) Table 4 lists the nomenclature, the La and Cu metal contents (obtained by ICP-OES), and the BET surface area of Ba 1−x La x Mn 0.7 Cu 0.3 O 3 (BMC-La x ) samples.According to the ICP-OES data, the percentage of Cu ranges from 7.1 wt% for BMC-La 0.6 to 9.8 wt% for BMC-La 0.3 , showing a wt% La from 5.4 wt% to 24.0 wt%.As seen in Table 4, the BET surface area of perovskites is lower than 10 m 2 g −1 , and these low surface areas are consistent with what is expected for solids with very low developed porosity such as perovskite-type mixed oxides [18,19].As indicated above, this is most likely due to the relatively high calcination temperature used during synthesis (850 • C) [20,21].The XRD patterns obtained for BMC-Lax samples are displayed in Figure 5, along with the BaMn 0.7 Cu 0.3 O 3 (BMC) perovskite used as a reference, and Table 5 contains the most important related data.All the identified peaks belong to a perovskite structure, and only for BMC-La 0.1 is a very small intensity peak corresponding to BaMn 2 O 3 (PDF number: 01-071-1325) detected as a minority phase.In addition, it is observed that as the percentage of lanthanum increases, the intensity of the XRD peaks corresponding to the polytype BaMnO 3 perovskite structure [21]-at 27.0 • , 30.9 • , 27.5 • , 41.5 • , 52.9  , respectively (PDF number: 01-082-1152).Note that the XRD peaks of La 0.93 MnO 3 phase are present with similar or higher intensity with respect to those of the polytype BaMnO 3 phase for the two samples with high lanthanum content; so, as the La percentage increases, the formation of this La-based perovskite is favored, becoming the main phase for BMC-La 0.6 .So, if the degree of substitution of Ba by La is higher than that corresponding to x = 0.1, the insertion of La seems to be more difficult.The coexistence of the hexagonal and polytype perovskite structures for low contents of lanthanum-based perovskite indicates that the presence of La in the lattice hinders the incorporation of copper, which causes the change from the polytype hexagonal structure [16,21].The average crystal sizes of the polytype BaMnO 3 phase, calculated by applying the Williamson-Hall method to the corresponding XRD peaks [22], and reported in Table 5, indicate that the addition of lanthanum reduces the average crystal size of the polytype structure, but, when the trigonal structure becomes relevant (so for BMC-La 0.3 and BMC-La 0.6 ), the trend changes, and the average crystal size increases with the lanthanum content.On the contrary, the lattice parameters, corresponding to the polytype structure for BMC and BMC-La 0.1 and to the trigonal structure for BMC-La 0.3 and BMC-La 0.6 , do not appreciably change with the La percentage.As for the BM-Cex series, the XRD refinement data, included in Table 5, confirm the above-described trend of the different crystalline phases with the increase in the La percentage.
of the polytype structure, but, when the trigonal structure becomes relevant (so for BMC-La0.3 and BMC-La0.6), the trend changes, and the average crystal size increases with the lanthanum content.On the contrary, the lattice parameters, corresponding to the polytype structure for BMC and BMC-La0.1 and to the trigonal structure for BMC-La0.3 and BMC-La0.6, do not appreciably change with the La percentage.As for the BM-Cex series, the XRD refinement data, included in Table 5, confirm the above-described trend of the different crystalline phases with the increase in the La percentage.Information regarding the surface composition and the oxidation state of the elements present on the surface (up to around 5 nm in depth) is obtained using the XPS technique.The spectra for O 1s, Mn 2p 3/2 , and Cu2p 3/2 transitions are displayed in Figure 6.
For perovskites, the O 1s spectrum (Figure 6a) could be deconvoluted into three peaks with maximum binding energies at around 528.5, 530.5, and 533.0 eV that correspond to [23][24][25]: (i) lattice oxygen (O L ); (ii) adsorbed oxygen species (named "O ads ", which includes surface carbonate (CO 3 2− ), hydroxyl groups (OH − ), peroxide (O 2 2− ) or superoxide (O 2− ) ions, and oxygen defect sites); and (iii) chemisorbed water (O H2O ).After the addition of La, the area under the different deconvoluted peaks seems to have been modified.To analyze the effect of the different amounts of La in the lattice oxygen, the values of the O L /(Ba + Mn + La) ratio have been calculated using the area under the O L peak and the area of the peaks for the cations present on the surface.As all experimental values included in Table 6 are lower than the corresponding nominal value for ABO 3 (1.5),this means that, as observed for BM-Cex samples, oxygen vacancies exist on the surface [23,24] of all perovskites.These vacancies are generated to achieve the neutrality of positive and negative charges on the surface of the samples because a defect in the positive charge exists due to the presence of Cu (II) and the coexistence of Mn(III) and Mn(IV) (see discussion below).Note that after the addition of La, the value only increases from 0.8 to 0.9, and it does not further change with the La percentage.So, the amount of lattice oxygen, and consequently, of oxygen vacancies, seems not depending on the increase in the La percentage in the samples.As was indicated above for the BM-Cex series, the assignment of the manganese oxidation states via XPS is a difficult task [25,44,45]; however, the raw data for the Mn 2p 3/2 spectra suggest their presence on the surface of Mn (III) and Mn (IV).Following the same pathway as for the Ce series (the asymmetric shape of the XPS signal and based on the Ponce et al. criteria for manganese-based perovskites [32]), the Mn 2p 3/2 spectra (Figure 6b) could be interpreted as follows: (i) the signal at the highest binding energy corresponds to the Mn (III) satellite peak; (ii) the peak at intermediated binding energy (around 642 eV) is assigned to Mn (IV); and (iii) the peaks at the lowest binding energy (around 641 eV) are also associated with Mn (III).So, it seems that Mn(III) and Mn(IV) also coexist on the surface of all BMC-La x samples.Note that the presence of Mn(III) on the surface implies that oxygen vacancies should exist (in order to achieve the neutrality of positive and negative charges on surface), as evidenced in the data for the O 1s transition discussed above.Also, just as observed for the BM-Cex series, as two deconvoluted peaks are found for Mn(III), it seems that different electronic environments exist, probably due to the existence of oxygen vacancies and/or copper species.The Mn(IV)/Mn(III) ratio, included in Table 6 and calculated using the area under the corresponding deconvoluted XPS peaks, reveals that Mn(IV) is the main oxidation state on the surface for BMC and BMC-La 0.1 as the Mn(IV)/Mn(III) ratio is higher than 1, but as the La percentage increases, the ratio becomes lower than 1; so, Mn(III) seems to be the main oxidation state for BMC-La 0.3 and BMC-La 0.6 .This trend could be expected due to the increase in the positive charge on the surface caused by the progressive substitution of Ba (II) by La (III), which seems to hinder the oxidation of Mn (III) to Mn (IV); so, Mn(III) is favored by the presence of La, becoming the main oxidation state at high La contents.
On the other hand, three peaks can be fitted for the Cu 2p 3/2 (Figure 6c) spectra, with binding energies at around 933.0, 934.5, and 940.0-943.0eV.According to the literature [21,31], these peaks are assigned to Cu(II) with strong (Cu(II) s ) and weak (Cu(II) w ) interaction with the perovskite surface for the two former, and to Cu(II) satellite peak for the latest.Upon using the area under the XPS signals for each metal, the Cu/(Ba + Mn + Cu) XPS ratio has been calculated.This value is compared in Table 6 with the nominal one in order to obtain information about the copper distribution.This is because, if the XPS ratio is lower than or similar to the nominal one, this means that copper has been inserted into the perovskite structure; and if it is higher, this implies that copper is being accumulated on the surface [21,31].According to the data, the distribution of copper is affected by the presence of La, as an increase in the Cu/(Ba + Mn+ Cu) XPS ratio is found.This finding agrees with the XRD data that suggest a lower degree of copper insertion into the perovskite structure (as polytype structure is disfavored); so, the accumulation of copper on the surface increases with the percentage of La.Additionally, the ratio of the copper species with different interactions with perovskite ( Cu(II) s Cu(II) W ) has been calculated considering the area under the corresponding deconvoluted peaks, and an increase with lanthanum content was also detected.Thus, even though the copper species have progressively accumulated on the surface, a strong interaction between these surface copper species and the perovskite is favored, presenting BMC-La 0.6 with the highest proportion of Cu(II) s and BMC with the lowest one.
H 2 -TPR tests were carried out to examine the reducibility of BMC-Lax samples, and the H 2 consumption profiles are presented in Figure 7, where they are compared with the corresponding MnO 2 and CuO (divided by 4 to obtain a similar peak intensity) used as references.As described above for the BM-Cex series, and considering the assignation of the peaks detected in the profile exhibited by the MnO 2 and CuO references (see previous section for BM-Cex characterization), the three reduction peaks detected in the H 2 -TPR profiles of BMC-Lax samples correspond to (i) the high-intensity peak at the low-temperature region (200-400 • C), to the reduction of Mn(IV) and Mn(III) to Mn(II) and also of Cu(II) to Cu(0) [18,43]; (ii) the second wide and very-low-intensity peak at intermediate temperature region (700-800 • C), to the desorption/reduction of oxygen species; and (iii) the third peak, which is almost inappreciable for this series but usually appears in perovskites at the highest temperature (900-1000 • C), to the reduction of bulk Mn (III).Note that the addition of lanthanum at x > 0.1 provokes an increase in the intensity of the main peak; so, there is an improvement in the reducibility of the BMC-La 0.3 and BMC-La 0.6 samples with respect to BMC and BMC-La 0.1 .Additionally, a more-defined peak is featured for the former samples, which, in depth, is more similar to the one shown by CuO reference.This finding agrees with the XPS results (Figure 6c) that reveal a higher proportion of surface copper for these two samples.Focusing our attention on the temperature for the maximum of this peak, it is lower than that observed for the CuO and MnO 2 references, revealing a synergetic effect between copper and manganese, which was previously found for other copper perovskites [31].However, the temperature of the maximum is higher in the presence of La, and it increases with the La percentage (from 266 to 279 and 303 • C for BMC-La 0.1 , BMC-La 0.3 , and BMC-La 0.6 versus 259 • C for BMC), suggesting that the presence of La decreases the Mn-Cu synergetic effect.The area under the hydrogen consumption profiles of Figure 7a was used to determine the experimental hydrogen consumption per gram of catalyst between 200 and 400 • C, which is compared in Figure 7b to the theoretical hydrogen consumption calculated considering the total reduction of manganese and copper-either as Mn(III) + Cu(II) (blue line) or Mn(IV) + Cu(II) (red line).Thus, it appears that the experimental H 2 consumption is close to the nominal Mn(III) + Cu(II) for BMC and BMC-La 0.1 , and, after increasing the lanthanum percentage in the BMC-La 0.3 and BMC-La 0.6 perovskites, it progressively increases until nearing the corresponding nominal Mn(IV) + Cu(II).This trend suggests an increase in the amount of bulk Mn(IV) with the increasing lanthanum percentage in perovskite.
Molecules 2024, 29, x FOR PEER REVIEW 13 of 21 references.As described above for the BM-Cex series, and considering the assignation of the peaks detected in the profile exhibited by the MnO2 and CuO references (see previous section for BM-Cex characterization), the three reduction peaks detected in the H2-TPR profiles of BMC-Lax samples correspond to (i) the high-intensity peak at the low-temperature region (200-400 °C), to the reduction of Mn(IV) and Mn(III) to Mn(II) and also of Cu(II) to Cu(0) [18,43]; (ii) the second wide and very-low-intensity peak at intermediate temperature region (700-800 °C), to the desorption/reduction of oxygen species; and (iii) the third peak, which is almost inappreciable for this series but usually appears in perovskites at the highest temperature (900-1000 °C), to the reduction of bulk Mn (III).Note that the addition of lanthanum at x > 0.1 provokes an increase in the intensity of the main peak; so, there is an improvement in the reducibility of the BMC-La0.3 and BMC-La0.6 samples with respect to BMC and BMC-La0.1.Additionally, a more-defined peak is featured for the former samples, which, in depth, is more similar to the one shown by CuO reference.This finding agrees with the XPS results (Figure 6c) that reveal a higher proportion of surface copper for these two samples.Focusing our attention on the temperature for the maximum of this peak, it is lower than that observed for the CuO and MnO2 references, revealing a synergetic effect between copper and manganese, which was previously found for other copper perovskites [31].However, the temperature of the maximum is higher in the presence of La, and it increases with the La percentage (from 266 to 279 and 303 °C for BMC-La0.1,BMC-La0.3, and BMC-La0.6 versus 259 °C for BMC), suggesting that the presence of La decreases the Mn-Cu synergetic effect.The area under the hydrogen consumption profiles of Figure 7a was used to determine the experimental hydrogen consumption per gram of catalyst between 200 and 400 °C, which is compared in Figure 7b to the theoretical hydrogen consumption calculated considering the total reduction of manganese and copper-either as Mn(III) + Cu(II) (blue line) or Mn(IV) + Cu(II) (red line).Thus, it appears that the experimental H2 consumption is close to the nominal Mn(III) + Cu(II) for BMC and BMC-La0.1, and, after increasing the lanthanum percentage in the BMC-La0.3 and BMC-La0.6 perovskites, it progressively increases until nearing the corresponding nominal Mn(IV) + Cu(II).This trend suggests an increase in the amount of bulk Mn(IV) with the increasing lanthanum percentage in perovskite.The information about oxygen mobility through the lattice is obtained from the O2-TPD tests [1,27,30], with the oxygen-evolved profiles for BMC-Lax being displayed in Figure 8.The samples do not evolve oxygen at temperatures lower than 650 °C, as only a The information about oxygen mobility through the lattice is obtained from the O 2 -TPD tests [1,27,30], with the oxygen-evolved profiles for BMC-Lax being displayed in Figure 8.The samples do not evolve oxygen at temperatures lower than 650 • C, as only a desorption peak between 650 and 900 • C is found, which corresponds to the release of β-O 2 ; that is, oxygen comes from the perovskite lattice linked to the reduction of Mn(IV)/Mn(III) and Cu(II) cations [41], which is favored by the presence of bulk oxygen vacancies.In the presence of lanthanum, an increase in the temperature for the maximum is detected (from 753 • C for BMC to 773, 779, and 773 • C for BMC-La 0.1 , BMC-La 0.3 , and BMC-La 0.6 , respectively).The shift towards higher temperatures should be a consequence of a decrease in the Mn-Cu synergetic effect, probably due to the lowering of the amount of Cu inside the structure.Note that the amount of β-O 2 evolved (calculated using the area under the peak between 650 • C and 900 • C) also increases with the La content from 49 to 91 µmol g −1 ; so, improved oxygen mobility seems to be provoked by the presence of La.This trend agrees with the increase in the reducibility previously observed during H 2 -TPR tests.
Molecules 2024, 29, x FOR PEER REVIEW 14 of 21 desorption peak between 650 and 900 °C is found, which corresponds to the release of β-O2; that is, oxygen comes from the perovskite lattice linked to the reduction of Mn(IV)/Mn(III) and Cu(II) cations [41], which is favored by the presence of bulk oxygen vacancies.In the presence of lanthanum, an increase in the temperature for the maximum is detected (from 753 °C for BMC to 773, 779, and 773 °C for BMC-La0.1,BMC-La0.3, and BMC-La0.6, respectively).The shift towards higher temperatures should be a consequence of a decrease in the Mn-Cu synergetic effect, probably due to the lowering of the amount of Cu inside the structure.Note that the amount of β-O2 evolved (calculated using the area under the peak between 650 °C and 900 °C) also increases with the La content from 49 to 91 µmol g −1 ; so, improved oxygen mobility seems to be provoked by the presence of La.This trend agrees with the increase in the reducibility previously observed during H2-TPR tests.

Soot Oxidation Tests
The temperature-programmed reaction in the presence of model soot (soot-TPR) was used to assess the catalytic performance of BM-Cex and BMC-Lax perovskites for GDI soot oxidation in the two gaseous mixtures (0% and 1% O2 in He) previously used [16].The soot conversion profiles are presented in Figure 9 for BM-Cex samples and in Figure 10 for BMC-Lax, being selective for CO2 (SCO2), and the T10% and T50% values (temperatures to achieve 10% and 50% of soot conversion, respectively) presented in Tables 7 and 8 for the BM-Cex and BMC-Lax series.
Figure 9a depicts the soot conversion profiles in the absence of oxygen for BM-Cex samples, where it is observed that all perovskites catalyze the soot oxidation (if they are compared with the profile obtained in the absence of catalyst), showing a shift of the soot conversion profile towards lower temperatures as the Ce content increases.In the presence of perovskites, the reaction seems to occur with the oxygen evolved from the samples, which is mainly β-O2, as the soot conversion is mainly promoted at temperatures higher than 650 °C (see Figure 4).Consequently, the temperature for soot conversion directly depends on the temperature at which the β-O2 starts to be evolved from the samples; that is, at T > 700 °C.From the BM-Cex series, BM-Ce0.6 is the most-active catalyst as it features

Soot Oxidation Tests
The temperature-programmed reaction in the presence of model soot (soot-TPR) was used to assess the catalytic performance of BM-Cex and BMC-Lax perovskites for GDI soot oxidation in the two gaseous mixtures (0% and 1% O 2 in He) previously used [16].The soot conversion profiles are presented in Figure 9 for BM-Cex samples and in Figure 10 for BMC-Lax, being selective for CO 2 (S CO2 ), and the T 10% and T 50% values (temperatures to achieve 10% and 50% of soot conversion, respectively) presented in Tables 7 and 8 for the BM-Cex and BMC-Lax series.reported that this phase presents a poor catalytic activity for soot oxidation [46].In conclusion, the increase in cerium content in the BM-Cex samples does not improve the catalytic performance of soot oxidation in 1% O2/H, as shown by BM-Ce0.1;consequently, this is the best catalyst.Thus, it seems that the similar amount of surface oxygen vacancies to BM raw perovskite and the highest proportion of Mn(IV) and Ce(IV) among all BM-Cex samples make BM-Ce0.1 the best catalyst.Regarding the soot conversion profiles presented in Figure 10, and the SCO2, T10%, and T50% data compiled in Table 8 for BMC-Lax samples, it seems that, independently of the presence of oxygen in the reaction atmosphere, the increase in the lanthanum content does not improve the catalytic performance of BMC-La0.1, even though BMC-La0.3 and BMC-La0.6 are able to catalyze the soot oxidation reaction, because they present lower T10% and T50% values and a higher SCO2 than that observed for the uncatalyzed reaction.Based on the characterization results, it seems that this trend is caused by the decrease in the amount of Mn(IV) with respect to BMC-La0.1, which does not seem to be compensated by the increase in the amount of surface Cu(II).
In summary, the increase in the amount of Ce (from x = 0.1 to x = 0.6) only improves the catalytic performance of the BM raw sample for soot oxidation if the oxygen coming from perovskite is uniquely available for soot oxidation, which seems to be due to the contribution of the Ce(IV)/Ce(III) redox pair to the lattice oxygen (β-O2) generation.Figure 9a depicts the soot conversion profiles in the absence of oxygen for BM-Cex samples, where it is observed that all perovskites catalyze the soot oxidation (if they are compared with the profile obtained in the absence of catalyst), showing a shift of the soot conversion profile towards lower temperatures as the Ce content increases.In the presence of perovskites, the reaction seems to occur with the oxygen evolved from the samples, which is mainly β-O 2 , as the soot conversion is mainly promoted at temperatures higher than 650 • C (see Figure 4).Consequently, the temperature for soot conversion directly depends on the temperature at which the β-O 2 starts to be evolved from the samples; that is, at T > 700 • C. From the BM-Cex series, BM-Ce 0.6 is the most-active catalyst as it features the highest soot conversion values at T > 700 • C. T 10% data in Table 7 evidence that BM-Ce 0.3 and BM-Ce 0.6 perovskites present the lowest T 10% values among the BM-Cex samples.Note that these two perovskites evolve a higher amount of oxygen during the O 2 -TPD tests than the BM-Ce 0.1 and BM raw samples, probably due to the contribution of Ce(IV)/Ce(III) reduction as they present a higher amount of Ce(IV), both on the surface (as revealed via XPS) and in the bulk (due to the presence of CeO 2 , as identified via XRD), than BM-Ce 0.1 and BM.
Figure 9b and the data in Table 7 present the soot-TPR profiles and the S CO2 , T 50% , and T 10% data for BM-Cex samples in a 1% O 2 atmosphere.In the presence of oxygen, it seems that only the introduction of the lowest amount of Ce (BM-Ce 0.1 ) allows us to improve the performance of the BM raw sample in terms of T 10% , T 50% , and S CO2 as, after increasing the Ce percentage, the role of the catalysts seems to be worse, as T 10% and T 50% values increase and S CO2 decreases in the BM-Ce 0.3 and BM-Ce 0.6 .In fact, BM-Ce 0.6 presents a significantly low catalytic activity, remaining so even under the uncatalyzed test at high temperatures.According to characterization data, this trend seems being related to (i) the lower amount of oxygen surface vacancies as cerium content increases (see XPS results in Table 3); (ii) the significant decrease in the amount of Mn(IV) on the surface (XPS) and in the bulk (H 2 -TPR); (iii) a lower reducibility (H 2 -TPR) for BM-Ce 0.3 and BM-Ce 0.6 with respect to BM-Ce 0.1 ; and (iv) the increasing amount of CeO 2 (see XRD patterns in Figure 1), as it has been reported that this phase presents a poor catalytic activity for soot oxidation [46].In conclusion, the increase in cerium content in the BM-Cex samples does not improve the catalytic performance of soot oxidation in 1% O 2 /H, as shown by BM-Ce 0.1 ; consequently, this is the best catalyst.Thus, it seems that the similar amount of surface oxygen vacancies to BM raw perovskite and the highest proportion of Mn(IV) and Ce(IV) among all BM-Ce x samples make BM-Ce 0.1 the best catalyst.
Regarding the soot conversion profiles presented in Figure 10, and the S CO2 , T 10%, and T 50% data compiled in Table 8 for BMC-La x samples, it seems that, independently of the presence of oxygen in the reaction atmosphere, the increase in the lanthanum content does not improve the catalytic performance of BMC-La 0.1 , even though BMC-La 0.3 and BMC-La 0.6 are able to catalyze the soot oxidation reaction, because they present lower T 10% and T 50% values and a higher S CO2 than that observed for the uncatalyzed reaction.Based on the characterization results, it seems that this trend is caused by the decrease in the amount of Mn(IV) with respect to BMC-La 0.1, which does not seem to be compensated by the increase in the amount of surface Cu(II).
In summary, the increase in the amount of Ce (from x = 0.1 to x = 0.6) only improves the catalytic performance of the BM raw sample for soot oxidation if the oxygen coming from perovskite is uniquely available for soot oxidation, which seems to be due to the contribution of the Ce(IV)/Ce(III) redox pair to the lattice oxygen (β-O 2 ) generation.
Finally, by comparing the catalytic performance in soot oxidation of the two tested series, BM-Cex and BMC-Lax, and in the two conditions used, the following conclusions are reached: (i) In the absence of oxygen in the reaction atmosphere (100% He), BMC-La 0.1 is the best catalyst, as copper is also able to catalyze the soot oxidation [47].(ii) If oxygen is present in the reaction atmosphere (1% O 2 /He), BM-Ce 0.1 is the most active catalyst as it presents a higher proportion of Mn(IV) than BMC-La 0.1 .
Thus, it can be concluded that the addition of an amount of Ce or La dopant higher than that corresponding to x = 0.1 in Ba 1−x Ce x MnO 3 and Ba 1−x La x Cu 0.3 Mn 0.7 O 3 does not allow us to improve the catalytic performance of BM-Ce 0.1 and BMC-La 0.1 for soot oxidation in the conditions tested.

Characterization
The perovskite samples were characterized using the following techniques: i.
ICP-OES to ascertain the actual percentage of elements: To carry out this analysis, 10 mg of sample were dissolved in 5 mL of aqua regia diluted in 10 mL of distilled water.The analysis was performed using an Optimal 4300 DV Perkin-Elmer instrument (Waltham, MA, USA).ii.
N 2 adsorption at −196 • C, employing an Autosorb-6B device from Quanta Chrome (Anton Paar Austria GmbH, Graz, Austria) to measure the BET surface area.iii.
XRD to determine the crystalline structure: The X-ray patterns were captured using a Bruker D8-Advance device (Billerica, MA, USA) using the Cu K α radiation (1.4506 Å) and a step rate of 0.4 • min −1 between 20 • and 80 • 2θ angles.On the other hand, the Williamson-Hall method has been employed as it allows for more accuracy in the calculation of the average crystal size because it discards the contribution of the lattice strain to the full width at half maximum (FWHM) of the XRD peaks [22].Finally, XRD refinement was performed to determine the percentage of the different crystalline phases in the sample [50] by using the HighScore Plus software (Malvern Panalytical B.V. Almelo, The Nertherlands, 4.9 (4.9.0.27512) version).iv.
XPS to evaluate the surface composition: An Al K α (1486.7 eV) radiation source and a Thermo-Scientific K-Alpha photoelectron spectrometer (Thermo-Scientific, Waltham, MA, USA) were used, and, to obtain the XPS spectra, the pressure within the analysis chamber was maintained at 5 × 10 −10 mbar.The spectrometer's peakfit software (Thermo Avantage v5.9929) was used to determine the binding energy (BE) and kinetic energy (KE) values.The C 1s transition was set at 284.6 eV.v.
H 2 -TPR for assessing the reducibility of samples.To develop the tests, 30 mg of sample were heated at 10 • C min −1 from 25 • C to 1000 • C and 40 mL min −1 of a gaseous mixture consisting of 5% H 2 /Ar were used.A CuO reference sample, which is reduced to Cu 0 , was employed to quantify the H 2 consumption.The tests were carried out in a Pulse Chemisorb 2705 (from Micromeritics, Norcross, GA, USA) outfitted with a Thermal Conductivity Detector (TCD).vi.
O 2 -TPD to estimate the oxygen evolved from samples, which informs about the mobility of oxygen.Using a Thermal Gravimetric-Mass Spectrometer equipment (TG-MS, Q-600-TA, and Thermostar from Balzers Instruments, (Balzers, Liechtenstein), 16 mg of sample was heated in a helium gas flow (100 mL min −1 ) at a rate of 10 • C min −1 to 950 • C. In order to remove the moisture, each sample was heated to 150 • C for one hour before the tests.The 18, 28, 32, and 44 m/z signals were

Figure 5 . 3 a
Figure 5. XRD patterns of the BMC and BMC-Lax samples.Table 5. XRD data.

Figure 9 .
Figure 9. Soot-TPR conversion profiles as a function of the temperature of BM and BM-Cex catalysts in 100% He (a) and in 1% O2/He (b).Figure 9. Soot-TPR conversion profiles as a function of the temperature of BM and BM-Ce x catalysts in 100% He (a) and in 1% O 2 /He (b).

Figure 9 .
Figure 9. Soot-TPR conversion profiles as a function of the temperature of BM and BM-Cex catalysts in 100% He (a) and in 1% O2/He (b).Figure 9. Soot-TPR conversion profiles as a function of the temperature of BM and BM-Ce x catalysts in 100% He (a) and in 1% O 2 /He (b).

Figure 10 .
Figure 10.Soot-TPR conversion profiles as a function of temperature of BMC and BMC-Lax catalysts in 100% He (a) and in 1% O2/He (b).

Figure 10 .
Figure 10.Soot-TPR conversion profiles as a function of temperature of BMC and BMC-La x catalysts in 100% He (a) and in 1% O 2 /He (b).

Table 1 .
BET surface area and cerium content of BM-Cex samples.

Table 3 .
XPS data of BM-Cex samples.

Table 3 .
XPS data of BM-Cex samples.

Table 4 .
BET surface area and lanthanum and copper content of BMC-Lax samples.

Table 6 .
XPS data of BMC and BMC-Lax.

Table 6 .
XPS data of BMC and BMC-Lax.

Table 7 .
T 10% , T 50% , and S CO2 for soot oxidation in the two tested atmospheres for the uncatalyzed system: BM and BM-Cex.

Table 7 .
T10%, T50%, and SCO2 for soot oxidation in the two tested atmospheres for the uncatalyzed system: BM and BM-Cex.

Table 8 .
T 10% , T 50% , and S CO2 for soot oxidation in the two tested atmospheres of BMC-La x catalysts.